Determination of martensite structures of the Au7Cu5Al4 ... · PDF file Determination of...
Embed Size (px)
Transcript of Determination of martensite structures of the Au7Cu5Al4 ... · PDF file Determination of...
Available online at www.sciencedirect.com
Acta Materialia 79 (2014) 234–240
Determination of martensite structures of the Au7Cu5Al4 and Au7Cu5.7Al3.3 shape-memory alloys
Margaret M. Elcombe a, Catherine S. Kealley b, Vijay K. Bhatia c, Gordon J. Thorogood d, Damien J. Carter e, Maxim Avdeev a, Michael B. Cortie c,⇑
a Bragg Institute, Australian Nuclear Science and Technology Organisation, Locked Bag 2001, Kirrawee DC, NSW 2232, Australia b John de Laeter Centre, Curtin University, GPO Box U1987, Perth, WA 6845, Australia
c Institute for Nanoscale Technology, University of Technology Sydney, PO Box 123, Broadway, NSW 2007, Australia d Institute of Materials Engineering, Australian Nuclear Science and Technology Organisation, Locked Bag 2001, Kirrawee DC, NSW 2232, Australia
e Nanochemistry Research Institute, Curtin University, GPO Box U1987, Perth, WA 6845, Australia
Received 11 April 2014; received in revised form 11 July 2014; accepted 16 July 2014 Available online 16 August 2014
The b-phase of Au7Cu5Al4 undergoes a reversible shape-memory phase transformation for which several conflicting martensite phases have been reported. Here we show the significance of the cooling temperature used to obtain the martensite. If Au7Cu5Al4 is cooled from the parent phase condition to cryogenic temperatures, e.g. below 200 K, the martensitic phase is orthorhombic (space group Pcmn, a = 4.4841 Å, b = 5.8996 Å, c = 17.8130 Å); however, when this composition is cooled to only �260 K it will in general consist of a mixture of orthorhombic and monoclinic phase (the latter has space group P21/m, a = 4.4742 Å, b = 5.9265 Å, c = 13.3370 Å, b = 91.425�). In contrast, a sample with decreased Al content (Au7Cu5.7Al3.3) transforms fully to monoclinic phase if cooled to �260 K. � 2014 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.
Keywords: X-ray diffraction; Neutron diffraction; Shape memory; Modulated martensite; Au–Cu–Al
The b-phase with approximate stoichiometry Au7Cu5Al4 is a shape-memory alloy (SMA) sometimes referred to as Spangold . Like other SMAs it undergoes a reversible, displacive, thermoelastic phase transformation between a parent (high-temperature) phase and a martensitic (low- temperature) phase . The alloy qualifies as 18 carat gold and therefore has been of minor interest in the jewelry industry ; however, its good castability, high strength and wear resistance, and resistance to corrosion [3,4] suggest that it could also be more generally useful as a SMA. One application might be as a component within
1359-6454/� 2014 Acta Materialia Inc. Published by Elsevier Ltd. All rights r
⇑ Corresponding author. Tel.: +61 2 9514 2208. E-mail address: firstname.lastname@example.org (M.B. Cortie).
biomedical devices since the high gold content of the alloy renders it radiopaque—a property that facilitates the posi- tioning or manipulation of a medical device in vivo .
Previously, the martensite start (Ms) temperature in this alloy has been reported in the range of 293–303 K and the austenite start (As) temperature in the range 328–353 K, with some variability due to the effect of thermal history [2,6–9]. The crystal structures of the parent and martensite phases are an important aspect of SMA technology, since they influence the nature of the transformations, the usable amount of strain, the reproducibility of the transformation temperatures and cyclic stability, all factors which must be controlled in technological applications of SMAs [10–12].
Recent work  has elucidated the structure of the b-phase at higher temperatures, showing that the parent phase possesses the L21 structure between the As and
http://dx.doi.org/10.1016/j.actamat.2014.07.039 mailto:email@example.com http://dx.doi.org/10.1016/j.actamat.2014.07.039 http://crossmark.crossref.org/dialog/?doi=10.1016/j.actamat.2014.07.039&domain=pdf
M.M. Elcombe et al. / Acta Materialia 79 (2014) 234–240 235
�903 K, and the B2 primitive cubic structure between �903 K and its melting point. It melts directly from the B2 structure into the liquid state.
Various structures have been proposed for the martens- ite phase of Au7Cu5Al4. For example, it was shown that the martensite could be considered to have a hexagonal-type packing arrangement on the B19 model, but with a unit cell of double size to account for the ternary ordering . In contrast, analysis of electron diffraction patterns indicated that it was monoclinic with a = 4.65 Å, b = 5.56 Å, c = 3.906 Å, a (sic) = 87� , which is similar to the heavily faulted structures determined for many Cu-base martens- ites. The endothermic transformation of the martensite to the parent phase at �350 K is clearly discernible on differ- ential scanning calorimetry or differential thermogravimet- ric traces; however, several workers have also published data showing that some martensite samples undergo an additional, less pronounced, transformation at �320 K, prior to their up-transformation to parent phase [8,9].
Recently, we became aware that the temperature to which a martensitic sample was cooled influenced its X-ray diffraction pattern. Here we have used in situ X-ray and neutron powder diffraction studies to show that there are both monoclinic and orthorhombic martensite structures in this system, with the nature of the martensite being controlled by the cooling temperature.
2.1. Sample manufacture
The samples for this project were manufactured by melt- ing high-purity base metals of Au (99.99%), Cu (99.9%) and Al (99.99 + %) in an alumina crucible under a protec- tive layer of carbon pellets.
The Au was melted first, and then the Cu and Al stirred in. The samples were annealed at 970 K to convert them into the b-phase, followed by quenching into iced brine. The structures obtained from two samples are reported here: Spangold, i.e. Au7Cu5Al4 (43.5, 32.2, 24.2 at.% gold, cop- per, aluminum), and Au7Cu5.7Al3.3 (43.3, 35.7, 20.9 at.% gold, copper, aluminum). In all our refinements, it has been assumed that all phases in a sample have the analyzed composition. Powders were prepared by wet grinding on abrasive paper, followed by washing in water. The individ- ual particle sizes were of the order of several tens of micrometers.
2.2. X-ray diffraction
X-ray powder diffraction was undertaken at the Euro- pean Synchrotron Radiation Facility (ESRF) (ID11: Mate- rials Science Beamline) and the Australian Synchrotron (AS) (10BM1: Powder Diffraction). In both cases spinning 0.3 mm capillaries filled with powdered sample were used. A LaB6 standard (NIST 660a) was used to calibrate the wavelength and determine the instrument contributions
to the observed line profiles. Powders were measured at temperatures ranging from 252 to 382 K. Due to the large grain sizes within the material and the small volume sam- pled within the silica capillaries, the XRD patterns obtained at either synchrotron were slightly affected by texture.
At the ESRF samples were analyzed at an incident wavelength of 0.31090 ± 0.00001 Å. A short wavelength was chosen in an attempt to minimize the impact of the absorption on the data. Due also to the small size of the beam at ESRF (100 lm � 100 lm), the sample was stepped along its length in 10 lm increments in order to improve counting statistics. Each camera image was radially aver- aged to give intensity vs. 2h (0.0187� per step). The mean of 360 patterns was used for structure refinement. The sam- ple was cooled to 200 K and data collected at 292 K.
At the AS wavelengths of 0.42654 ± 0.00001 Å 0
(sample Au7Cu5Al4) and 1.1597 ± 0.00001 Å (sample Au7Cu5.7- Al3.3) were applied. Samples Au7Cu5Al4 and Au7Cu5.7Al3.3 were precooled to either liquid nitrogen (77 K) or 263 K and the data subsequently collected at room temperature (Mythen strip detector, 0.004� intervals).
2.3. Neutron diffraction
Complementary neutron powder diffraction (NPD) data were collected on Echidna (the high-resolution powder dif- fractometer) at the OPAL reactor of the Australian Nuclear Science and Technology Organisation (ANSTO). The configuration of this instrument has been described by Liss et al. . Neutron diffraction data is useful because it is more sensitive to the Al positions in this system and because it samples a much greater volume of material. (The latter factor helps eliminate texture effects.) Data were collected from stationary powder samples at 302 K using neutron wavelengths of 2.2736 and 2.4380 Å from the (331) reflection of the germanium monochromator; no extra collimation was used. Approximately 0.3 cm3 of the powder was packed into a vanadium can with a 6 mm diameter. Al2O3 standard patterns were also collected for each instrumental configuration.
2.4. Rietveld refinement
The structures were determined by co-refinement of the full X-ray and neutron diffraction patterns using the pro- gram Rietica [16,17]. In the combined XRD–NPD Rietveld analysis the AS was down-weighted to 40% to compensate for much higher counting statistics than that of the NPD data. The parameters refined included relative scale factors between the data sets, wavelengths and zeroes (to allow for the slight temperature differences between the various mea- surements), instrument parameters for each data set, and crystal structural parameters with isotropic displacement parameters (assumed as the same for all phases). The refined Pcmn, cubic and P21/m structures wer